Carbohydrate Polymers 117 (2015) 286–296
Contents lists available at ScienceDirect
Carbohydrate Polymers journal homepage: www.elsevier.com/locate/carbpol
Tunicate cellulose nanocrystals: Preparation, neat ﬁlms and nanocomposite ﬁlms with glucomannans Yadong Zhao, Yujia Zhang, Mikael E. Lindström, Jiebing Li ∗ Department of Fibre and Polymer Technology, Royal Institute of Technology, KTH, Teknikringen 56-58, SE-100 44 Stockholm, Sweden
a r t i c l e
i n f o
Article history: Received 21 February 2014 Received in revised form 4 May 2014 Accepted 12 September 2014 Available online 22 September 2014 Keywords: Tunicate cellulose Ciona intestinalis Nanocrystals Konjac glucomannan Spruce glucomannan Nanocomposite ﬁlms
a b s t r a c t Cellulose nanocrystals (CNs) were prepared from tunicate by enzymatic hydrolysis (ECN), TEMPOmediated oxidation (TCN) and acid hydrolysis (ACN). They were cast alone or blended with glucomannan (GM) from konjac or spruce to prepare ﬁlms. Different CNs were obtained with a yield of ECN > TCN > ACN with corresponding order of decreased Mw but increased crystallinity. The CNs’ diameters were on the nanometre scale, with lengths of ECN > TCN > ACN. For CN-ﬁlms, TCN and ACN ﬁbrils were stretched and parallel to each other due to surface charges. For CN–GM ﬁlms, both components interacted strongly with each other, resulting in changes of crystallinity, speciﬁc surface area, ﬁbril diameter and contact angle compared with CN ﬁlms. The composite ﬁlms had good thermal, optical and mechanical properties; the last ones are apparently better than similar ﬁlms reported in the literature. This is the ﬁrst systematic study of different tunicate CN–GM nanocomposite ﬁlms and the ﬁrst ever for spruce GM. © 2014 Elsevier Ltd. All rights reserved.
1. Introduction In recent years, renewable, sustainable and environmentally friendly materials have gained much attention for science and technology development. Among all natural polymers, cellulose is considered to be one of the most promising materials due to its abundant availability in nature and its excellent renewability. Its inherent ﬁbrous and crystal structure makes cellulose attractive for various potential material applications, such as ﬁlms or composites, due to its high strength, stiffness, transparency and protective barrier. Speciﬁcally, cellulose is a good candidate for substituting synthetic polymers for food applications, such as packaging and other food contact surfaces (Sorrentino, Gorrasi, & Vittoria, 2007). Because cellulose is nontoxic and biodegradable, it is particularly advantageous for these applications. For example, cellulose-based
Abbreviations: TC, tunicate cellulose; CN, cellulose nanocrystal; ECN, CN from enzymatic hydrolysis; TCN, CN from TEMPO-mediated oxidation; ACN, CN from acid hydrolysis; GM, glucomannan; KGM, konjac glucomannan; SGM, spruce glucomannan; EKG20, composite ﬁlm with ECN and 20% KGM; TKG20, composite ﬁlm with TCN and 20% KGM; AKG20, composite ﬁlm with ACN and 20% KGM; CSG10, composite ﬁlm with regenerated TC and 10% SGM; ESG20, composite ﬁlm with ECN and 20% SGM; TSG20, composite ﬁlm with TCN and 20% SGM; ASG20, composite ﬁlm with ACN and 20% SGM; CKG10, composite ﬁlm with regenerated TC and 10% KGM. ∗ Corresponding author. E-mail address: [email protected]
(J. Li). http://dx.doi.org/10.1016/j.carbpol.2014.09.020 0144-8617/© 2014 Elsevier Ltd. All rights reserved.
edible ﬁlms have been tested for packaging fresh beans and strawberries (Ayranci & Tunc¸, 1997). Regenerated cellulose ﬁlms are biodegradable in soil (Zhang et al., 1996). However, the primary issues remain concerning cellulose applications: processing, performance and cost (Sorrentino et al., 2007). Distinctly, cellulose has very low ﬁlm formation processability due to its poor dissolution and suspension properties in water. To prepare high performance ﬁlms or biocomposites, good dispersion in an aqueous solution during processing and strong interactions in the ﬁnal structures are important. For decades, the degradation of cellulose into nanoscale particles, termed cellulose nanocrystals (CNs), has been an effective means of modifying cellulose. After size reduction, with or without the introduction of surface charge, a CN can be suspended in aqueous solution, improving its processability. In addition, due to its nanometre-size after dispersion, markedly improved mechanical, thermal, barrier and other physio-chemical properties can be obtained for CN ﬁbril ﬁlms and composites compared to untreated cellulose. In the literature, there are many synonyms used to describe the CNs used in this study, including cellulose microcrystals, whiskers, nanoparticles, microcrystallites, nanoﬁbres, or nanowires. A detailed description of CNs and the ﬁeld in general may be found in numerous reviews (Azizi Samir, Alloin, & Dufresne, 2005; de Souza Lima & Borsali, 2004; Fleming, Gray, & Matthews, 2001; Habibi, Lucia, & Rojas, 2010; Klemm, Heublein, Fink, & Bohn, 2005; Moon, Martini, Nairn, Simonsen, & Youngblood, 2011; Peng, Dhar, Liu, & Tam, 2011) and textbook (Kimura & Itoh, 2007).
Y. Zhao et al. / Carbohydrate Polymers 117 (2015) 286–296
CNs are prepared by various physical and chemical methods, among which acid hydrolysis is the most common (Anglès & Dufresne, 2000; Chang, Wang, Hung, & Perng, 2010; Jiang & Hsieh, 2013). Other methods include mechanical reﬁning (Jiang & Hsieh, 2013), TEMPO-mediated oxidation (Habibi, Chanzy, & Vignon, 2006; Okita, Fujisawa, Saito, & Isogai, 2010a) and enzymatic hydrolysis-assisted mechanical treatment (Henriksson, Henriksson, Berglund, & Lindström, 2007), and these methods produce a suspension of rod-like whiskers whose dimensions depend on the pretreatment method and cellulose origin (de Souza Lima & Borsali, 2004). In principle, the acid hydrolysis can not only remove the amorphous part and shorten the length of the cellulose ﬁbrils, but also introduce charged sulfate groups to the cellulose surface, and increase thus the dispersion ability of the CN in water (Revol, Bradford, Giasson, Marchessault, & Gray, 1992). However, it has also disadvantages, such as that the sulfate moieties at the CN surfaces are labile which can be readily removed with mild alkaline treatment (Habibi et al., 2006). The TEMPO-mediated oxidation converts the hydroxyl groups at the surface of the cellulose into charged carboxyl groups without the liability problem as the sulfate groups (Okita, Saito, & Isogai, 2010b). However, both methods are based on chemical reactions. An enzymatic hydrolysis is a totally bio-based treatment, which has advantages from the environmental point of view when compared with the chemical methods (Henriksson et al., 2007). To our best knowledge, it is rare that all these three methods were used and comprehensively compared in one study. Among all natural cellulose sources, tunicate is the only animal species that produces cellulose in the outer tissues, termed tunic, from which a puriﬁed fraction termed tunicin can be obtained (Hirose, Kimura, Itoh, & Nishikawa, 1999). Similar to plant cellulose, tunicate cellulose (TC) in the tunic aggregates in the form of microﬁbrils composed of a nearly pure cellulose I␤ allomorph (Kimura, Ohshima, Hirose, Nishikawa, & Itoh, 2001). TC has a very large aspect ratio (length = 100 nm to several micrometres and width = 15–30 nm); thus, the aspect ratio is between 3 and 67 (Peng et al., 2011). TC also has a high speciﬁc surface area (150–170 m2 /g), a high crystallinity (95%) and a reactive surface due to the presence of hydroxyl groups, which are important for its excellent mechaniˇ Davies, & Eichhorn, 2005). Therefore, TC is cal properties (Sturcová, an excellent candidate for CN preparation and for ﬁlm or composite ﬁlm applications. For example, a tunicin whisker/plasticised starch nanocomposite material has been developed (Anglès & Dufresne, 2000, 2001). When producing CN-based biodegradable ﬁlms, synthetic plasticisers are commonly used to further improve their chemical or physical properties, but it was found that for a low molecular weight plasticiser, the plasticiser was easily lost during utilisation, leading to contamination. A better method to achieve this goal is the incorporation of high molecular weight synthetic or natural polymers with cellulose to improve plasticity. Epoxy polymer (Ruiz, Cavaillé, Dufresne, Graillat, & Gérard, 2001), chitosan (Fernandes et al., 2010), starch (Teixeira et al., 2009), xylan (Stevanic, Bergström, Gatenholm, Berglund, & Salmén, 2012), latex (Favier et al., 1995) and PHA latex (Dufresne, Kellerhals, & Witholt, 1999) have been tested. In some cases, the role of CNs is simply to serve as a ﬁller in ﬁlms (Veigel, Müller, Keckes, Obersriebnig, & Gindl-Altmutter, 2011). A structural analogue to cellulose, glucomannan (GM), is another biopolymer consisting of ␤-1,4 linked mannose and glucose residues. Due to its low isolation cost, renewability and biodegradability, GM is an attractive candidate to replace traditional artiﬁcial polymers (Persson, Nordin, Zacchi, & Jonsson, 2007). Konjac is a well-known source for GM and konjac glucomannan (KGM) has commonly a weight average molecular weight of 1.088 × 106 (Li & Xie, 2006) and a mannose to glucose ratio of 1.51:1 (Yuan, Wu, Zhao, Wu, & Li, 2003). Spruce is another GM-rich source. There are two types of GMs in spruce depending
on the galactose content. The spruce glucomannan (SGM) used in this study is the galactose-poor GM and has lower weight average molecular weight (1.0 × 104 ) and higher mannose to glucose ratio (3.75:1) compared with the KGM (Zhang, Li, Lindström, Stepan, & Gatenholm, 2013). Generally, all mannan-based polysaccharides will interact well with cellulose (Whitney, Brigham, Darke, Reid, & Gidley, 1998), allowing for the production of good composite ﬁlms from CN and GM blends. In the literature, spruce galactoglucomannan, the galactose-rich GM, and KGM have been used to produce composite ﬁlms with woody cellulose nanowhiskers (Mikkonen et al., 2010). The aim of this study was to investigate the performance characteristics, such as high optical and thermal stability, mechanical strength and barrier function, of biodegradable and edible ﬁlm materials constructed from tunicate CNs with or without the addition of GM to further modify ﬁlm microstructure and physical properties. Three different preparations of tunicate CNs, enzymatic treatment, TEMPO-mediated oxidation and acid hydrolysis, were applied, and two GMs, KGM and SGM, were included in the study. To our knowledge, this is speciﬁcally the ﬁrst study to report the preparation, structure and high mechanical strength of different tunicate CNs in one study and their forming nanocomposite ﬁlms with GM and the ﬁrst ever using SGM in the ﬁeld. 2. Experimental 2.1. Materials TC was prepared and characterised from Ciona intestinalis in our laboratory (Zhao & Li, 2014). Food additive grade KGM (Mw of 1000k) was purchased from Hubei Konson Konjac Gum Co., Ltd, China. SGM (Mw of 10k) was extracted and puriﬁed from spruce (Picea abies) holocellulose in our laboratory, as described previously (Zhang et al., 2013). After analysis, the two GMs were found also differing in their mannose:glucose ratio (3.75 for SGM and 1.46 for KGM). Endoglucanase (Novozym 476) was purchased from Novozymes AS (Denmark) and used without further puriﬁcation. All reagents were of analytical grade, and they were obtained from VWR International AB, Stockholm, Sweden. 2.2. Preparation of CNs 2.2.1. Enzymatic hydrolysis A 0.5% cellulose suspension in phosphate buffer (pH 5) was prepared. After the addition of Novozym 476 (20 FPU/g), the mixture was incubated at 50 ◦ C for 2 h with shaking manually once every 30 min. The Novozym 476 in the reaction system was then denatured at 80 ◦ C for 30 min. Next, the treated cellulose was recovered by vacuum ﬁltration and washed several times with deionised water (Henriksson et al., 2007). Finally, the tunicate CN was dispersed in deionised water to produce a 0.5% suspension, which was then subjected to homogenisation using an IKA T-25 ULTRA-TURRAX Digital Homogeniser at 15000 rpm for 2 min and ultrasonication (Unique Sonicator, 40 kHz) for 1 min in an ice-bath to yield a homogeneous CN suspension, termed ECN. 2.2.2. TEMPO-mediated oxidation Cellulose (0.5 g) was suspended in water (100 ml) containing TEMPO (0.016 g, 0.1 mmol) and sodium bromide (0.1 g, 1 mmol). The cellulose suspension was stirred continuously at 400–500 rpm. Then, 3.1 ml aqueous NaClO solution (12%, ∼1.61 M, made from the commercial NaClO with a commercially described 10–15% available amount of chlorine) was added drop-wise, so the total addition of NaClO was ∼5 mmol, equivalent to 10 mmol per gram of cellulose (Okita et al., 2010b). The pH of the reaction system was controlled at 10.0 ± 0.1 via the addition of 0.5 M NaOH. The reaction reached
Y. Zhao et al. / Carbohydrate Polymers 117 (2015) 286–296
completion when no further change in pH was observed, and it was fully quenched by the addition of 100 ml of ethanol (Okita et al., 2010a). The oxidised cellulose was recovered by vacuum ﬁltration and washed several times with ultrapure water to obtain a neutral pH. Then, a 0.5% homogeneous suspension of the TEMPO-mediated oxidised cellulose ﬁbres in water was prepared as mentioned above using the blender-type homogeniser at 15,000 rpm for 2 min, followed by ultrasonication for 1 min to produce TCN. 2.2.3. Acid hydrolysis A 0.5% cellulose suspension was prepared in 55% (v/v) H2 SO4 solution and hydrolysed at 60 ◦ C for 20 min with vigorous stirring. Then, the suspension was subjected to high-speed centrifugation (20,000 × g) for 15 min, and the precipitate was washed three times with 100 ml of deionised water by re-dispersion and recentrifugation (Anglès & Dufresne, 2000). Finally, the tunicate CN was dispersed in the deionised water to produce a 0.5% suspension, which was homogenised and sonicated to form the CN suspension as mentioned above, termed ACN. 2.3. Preparation of neat CN ﬁlms and CN–GM composite ﬁlms The CNs prepared above were directly cast on Petri dishes (15 ml with ∼75 mg solid content onto a 21 cm2 area) and dried at 50 ◦ C overnight to make neat CN ﬁlms. The thickness of the ﬁlms was approximately 10–20 m. For CN–GM composite ﬁlms, a 0.5% KGM or SGM solution/suspension was prepared by adding KGM or SGM in deionised water at 80 ◦ C. The composite ﬁlms were then prepared by adding the designated amount of CN to KGM or SGM. After mixing the KGM/SGM with the aqueous CN suspension by magnetic stirring at 80 ◦ C for 5 min, the mixed suspension was cast on Petri dish to obtain ﬁlms (15 ml with ∼75 mg solid content onto a 21 cm2 area). The ﬁlms were dried at 50 ◦ C overnight. The resulting ﬁlms (10–20 m thick) were termed AKG or ASG, EKG or ESG and TKG or TSG, followed by a number indicating the GM addition percentage after blending ACN, ECN and TCN, respectively, with KGM or SGM. For example, EKG 20 denotes an ECN–KGM ﬁlm made by blending 80% ECN and 20% KGM. As a reference experiment, the starting TC was immersed in ionic liquid containing 1-butyl-3-methylimidazolium chloride (BmimCl) and stirred at 90 ◦ C for at least 3 h (until dissolved) to prepare a 0.5% solution, and KGM/SGM was also dissolved in BmimCl to prepare a 0.5% solution. The obtained solutions were mixed to produce blend mixture solutions having different TC to GM mass ratios, as described previously. The blend mixture solutions were stirred energetically for more than 3 h, degassed at 60 ◦ C, and spread over a Petri dish to form a ﬁlm (15 ml with ∼75 mg solid content onto a 21 cm2 area). The Petri dish covered with the blend solution was coagulated with distilled water until the ﬁlm detached. The detached ﬁlm was immersed in running water for over 12 h and then dipped in deionised water three times (over 3 h every time) with slight stirring to completely remove BmimCl. Finally, the transparent ﬁlms were dried at 50 ◦ C overnight, and they were named CKG or CSG, followed by a GM addition percentage number. 2.4. Characterisation methods 2.4.1. Size exclusive chromatography (SEC) analysis First, TC and CNs (30 mg) were activated with 30 ml of deionised water at 4 ◦ C for 1 h, and the excess water was removed by ﬁltration. Next, solvent-exchange with methanol (30 ml) was applied three times, followed by N,N-dimethylacetamide (DMAc) (30 ml) for 30 min. The activated samples were then dissolved in 8% LiCl/DMAc to reach a concentration of 0.8% of the sample weight by stirring at 4 ◦ C for 5 days, and the solutions were diluted with DMAc to
reach a ﬁnal concentration of 0.5% with respect to sample weight. The SEC system was equipped with a Rheodyne injector, a DGU20A3 degasser, a LC-20AD liquid chromatography system and a RID-10A refractive index detector. The separations were achieved using four 20 m Mixed-A columns with a guard column. The injection volume was 100 l, and the separations were performed at 80 ◦ C with the ﬂow rate of 0.5 ml/min of 0.5% LiCl/DMAc. Calibration was conducted with pullulan standards of nominal masses ranging from 320 to 800 kDa (Fluka/Riedel-de Haën, Seelze, Germany). Data acquisition and analysis was performed using LC Solution software (Shimadzu, Kyoto, Japan) equipped with the SEC system. 2.4.2. Morphological analysis Before scanning electron microscopy (SEM) analysis, all samples were coated with gold using a Cressington 208HR high-resolution sputter coater. A Cressington thickness monitor controller was used to control the thickness (3–5 nm). Then, sample morphology was analysed using a Hitachi S-4800 Field Emission Scanning Electron Microscope. The morphology of the cellulose nanocrystals was imaged with tapping-mode AFM (Multimode IIIa, Veeco, Santa Barbara, CA). The AFM images were recorded under ambient and air conditions (23 ◦ C and 50% relative humidity). RTESP silica cantilevers (Veeco) having a tip with a radius of 8 nm and a spring constant of 40 N/m oscillated at their fundamental resonance frequencies between 200 and 400 kHz. 2.4.3. Z-potential determination The zeta potential of the cellulose suspensions was measured using a Zetasizer Nano Z system (Malvern Instruments, UK). A nanocrystalline cellulose suspension (0.05%), previously sonicated for 5 min, was prepared and analysed to determine the zeta potential of the CN suspensions. 2.4.4. Thermo gravimetric analysis (TGA) Thermo gravimetrical analysis was collected using a Mettler Toledo TGA/SDTA 851e equipped with STARe software for data analysis. The samples were subjected to a heating scan between 30 and 800 ◦ C, with a rate of 10 ◦ C/min under an inert atmosphere of nitrogen at a gas ﬂow of 50 ml/min. 2.4.5. Fourier transform infrared spectroscopy (FTIR) analysis Fourier transform infrared spectra were obtained using a PerkinElmer Spectrum 2000 FTIR spectrometer (Waltham, MA, USA) equipped with an ATR system, Spectac MKII Golden Gate (Creecstone Ridge, GA, USA). The samples were analysed at wavelengths ranging from 600–4000 cm−1 . All spectra were obtained from dry samples subjected to 16 scans at a resolution of 4 cm−1 and an interval of 1 cm−1 at room temperature. Before data collection, background scanning was performed for background correction. Dynamic FTIR (Fourier transform infrared) spectra were recorded on a Varian 680-IR spectrometer (Varian Inc., Santa Clara, CA, USA) in transmission mode with a liquid nitrogen cooled MCT (Mercury Cadmium Telluride) detector. Thin ﬁlms were mounted between two parallel jaws in a specially constructed polymer modulator (PM-100) which was placed in a temperature control system (TC100) (MAT-Manning Applied Technology Inc., Troy, ID, USA). A modular humidity generator (MHG-32) (Projekt Messtechnik, Ulm, Germany) was connected to the TC-100. The average in-phase and out-of-phase spectra were made and normalised as described in detail in the literature (Stevanic et al., 2012). 2.4.6. X-ray diffraction (XRD) analysis A PANalytical X’Pert PRO Materials Research Diffractometer equipped with an X’Celerator detector was used to determine
Y. Zhao et al. / Carbohydrate Polymers 117 (2015) 286–296
the crystallinity index (CI) of the samples. The analysis was performed using monochromatic CuK␣ radiation at 30 mA and 40 kV. CI, deﬁned to evaluate the crystallinity of the different samples, was calculated using the following equation: CI =
I200 − Iam × 100 I200
where I200 is the intensity of the 200 lattice plane at 2 = 22.8◦ , and Iam is the intensity from the amorphous phase at approximately 2 = 18◦ (Reddy & Yang, 2005). 2.4.7. Speciﬁc surface area analysis The analysis was conducted by measuring the gas adsorption properties of the sample for which a BET-analysis was performed. First, approximately 0.1 g of sample was heated and degassed at 115 ◦ C under a vacuum for >300 min, removing all foreign adsorbed molecules. Then, controlled amounts of an inert gas (nitrogen) were introduced and adsorbed. At the temperature of liquid nitrogen (−196 ◦ C), the sample was exposed to varying pressures to generate adsorption isotherms. Adsorbed amounts were determined by the pressure variations due to adsorption by the sample. A Micrometritics ASAP 2020 Surface Area and Porosity Analyzer (Micromeritics, USA) and its software were used. 2.4.8. Contact angle determination The contact angle (CA) was determined by the pendant drop method with a water drop and an optical contact angle meter SL 100B from Solon Information Technology Co., Ltd. (Shanghai, China) at a relative humidity (RH) of 50% and 23 ◦ C. To compare different samples, each contact angle was taken at 45 s, and the average value of at least three measurements was used. 2.4.9. UV–vis transmittance determination The percent light transmission (T%) of the ﬁlms was monitored using Shimadzu UV-240 (Japan) equipment. To compare different samples, readings were taken at a wavelength of 600 nm. Film specimens were cut into rectangles and placed in a spectrophotometer test cell directly, and air was used as the reference. Transmittance was used to deﬁne the transparency of a measured ﬁlm. Due to the differences in the ﬁlm thicknesses, a normalisation procedure was followed to obtain normalised transmittance by thickness from normalised A* according to Beer–Lambert law using A∗ = A ×
where A is the observed absorbance at the ﬁlm thickness (m) of l for the ﬁlm concerned while la (13.2 m) is the average thickness for all prepared ﬁlms in this study. That is to say all the transmittances for ﬁlms were normalised with the same thickness of 13.2 m and then compared directly. 2.4.10. Mechanical strength measurement The tensile strength and Young’s modulus of the ﬁlms were determined using an Instron 4411 mechanical property tester with a 500-N load cell (Instron Ltd., Norwood, MA, USA). The initial grip distance was 25 mm, and the rate of grip separation was 5 mm/min. Two ﬁlms of each type and three specimens from each ﬁlm were tested. The specimens were 5 mm wide and approximately 60 mm long. The thickness of the specimens was measured at three points using a micrometer (NSK, Japan). 2.4.11. Conductometric titration The total carboxyl group content of TCN was determined by conductimetric titration according to SCAN-CM 65:02 standard with some modiﬁcations as described by other researchers (Araki, Wada,
& Kuga, 2000; Habibi et al., 2006; Rusli, Shanmuganathan, Rowan, Weder, & Eichhorn, 2011). Brieﬂy, TCN (100 mg) was suspended in 50 ml of 0.01 M HCl solutions containing 0.01 mM NaCl. After stirring for 10 min, the suspensions were titrated with 0.01 M NaOH. The conductometric titration was performed three times and the average value was used. Finally, the amount of the carboxyl groups was calculated by the following equation:
Ct × V × 106 m
where X is the total carboxyl group content (mol/g), Ct is the NaOH concentration (mol/l), V is the amount of NaOH (l) consumed corresponding to the plateau region and m (g) is the weight of the CN in the water suspensions. The similar conductometric titration was used to determine the acidic group content of ACN ( OSO3 − ) without HCl addition. Brieﬂy, 100 mg ACN was suspended in 50 ml of 0.01 mM NaCl and poured into a 100 ml three-necked round-bottomed ﬂask. Then, the mixture was stirred continuously for 10 min. The suspension was titrated using 0.002 M sodium hydroxide. The surface charges ( OSO3 − ) were calculated from the same equation above though the V here is the volume of NaOH (l) consumed before conductivity increase (Rusli et al., 2011). This method was also used to determine the total acidic groups of ECN.
3. Results and discussion 3.1. CN preparation The starting TC prepared from Ciona intestinalis consisted of large molecules, with an Mw of 7.31 × 105 and a polydispersity index (PDI) of 11.1 (Table 1). The morphology of the TC was similar to its natural form in the original animal in terms of cellulose ﬁbre structure, displaying long cellulose chains tightly packed together in crystallites, stabilised by strong and very complex intra and inter molecular hydrogen bonds, termed cellulose microﬁbrils. Due to its high molecular mass and compact morphological structure, TC was not soluble or able to be suspended in water. In this study, we utilised the three preparation methods mentioned above, i.e. enzymatic treatment, TEMPO-mediated oxidation and acid hydrolysis to produce CNs from TC to improve its dispersion in water and its ability to be processed using an aqueous solution via molecular mass and morphological size reduction, with or without the introduction of surface charge. Morphologically, amorphous and crystalline regions were present in the cellulose microﬁbrils. The crystalline regions are so compact that almost no crystal structure modiﬁcations took place at these regions. For enzymatic hydrolysis, Novozym 476, an endoglucanase, was used, which mainly attacked the amorphous regions to shorten the cellulose chains by hydrolysis. TEMPOmediated oxidation occurred mainly via oxidation of the CH2 OH groups at the C6 position, preferably in the amorphous region, which facilitated the mechanical disintegration of the cellulose after the oxidation, resulting in a gentle shortening of the cellulose chains and the introduction of charged carboxylic groups. Sulphuric acid induced a strong hydrolysis that removed a portion of the microﬁbrils by disrupting the amorphous regions surrounding the embedded parts within the cellulose microﬁbrils while leaving the microcrystalline segments intact. Simultaneously, charged surface sulphate esters were generated. Comparatively, enzymatic hydrolysis was the mildest (73.4% recovery yield), followed by TEMPO-mediated oxidation (62.8% recovery yield) and acid hydrolysis (30.0% recovery yield) (Table 1).
Y. Zhao et al. / Carbohydrate Polymers 117 (2015) 286–296
Table 1 Recovery yield, molecular mass, size, zeta potential and charged group content of the tunicate cellulose nanocrystals (CNs) compared to starting tunicate cellulose (TC).
Recovery yield (%) Molecular mass Mw Mn PDI Size Width (nm) Length (nm) Zeta potential (mV) Charged group content (mol/g)
731,000 66,000 11.1
46,300 29,200 1.58
30,900 21,800 1.42
5750 2170 2.65
16.04 ± 0.64 Several micrometres – –
17.1 ± 2.7 Several micrometres −7.48 13.6
15.9 ± 2.0 1590 ± 759 −40.3 428
20.0 ± 2.8 694 ± 312 −18.3 68.3
3.2. CN structures The molecular mass of the CNs after enzymatic treatment, TEMPO-mediated oxidation and acid hydrolysis decreased, with ECN > TCN > ACN (Mw of 4.63 × 104 , 3.09 × 104 and 5750, respectively). Due to structural modiﬁcations, the PDI decreased to 1.42–2.65, indicating that the CNs had more uniform molecular mass distributions compared to the starting TC (Table 1). FTIR analysis revealed that all CNs showed typical cellulose structural characteristics (Fig. 1(A)), with O H, C H and C O stretching vibrations at 3334 cm−1 , 2901 cm−1 and 1057 cm−1 , respectively. The peak at 1638 cm−1 was associated with the O H bending vibration of absorbed water. For ECN, the peak near 1738 cm−1 represented the presence of carbon atoms in various oxygen environments (Łojewska, Mi´skowiec, Łojewski, & Proniewicz, 2005). For TCN, the pronounced peak at 1609 cm−1 indicated an asymmetrical carboxylate COO− vibration overlapping with the O H bending vibration of the absorbed water (Jiang & Hsieh, 2013), verifying the presence of charged carboxyl groups introduced by TEMPO-mediated oxidation. Here, the absolute vibration frequency was dependent on the status of the functional groups (Łojewska et al., 2005). For ACN, the signiﬁcant peak near 1160 cm−1 conﬁrmed the presence of charged
sulphate ester bonds on the cellulose chains generated by sulphuric acid hydrolysis (Chang et al., 2010). The contents of charged groups on the CNs were determined by conductometric titrations of aqueous CNs suspensions. The results showed that TCN exhibited a carboxyl group content of 428 mol/g (Table 1), which agrees quite well with the 300–500 mol/g reported by Besbes, Alila, and Bouﬁ (2011). It was followed by ACN with a charged group ( OSO3 − ) content of 68.3 mol/g, which was slightly lower than the 85 mol/g reported by Rusli et al. (2011). It is reasonable to ﬁnd out the lowest charged group content (13.6 mol/g) for ECN due to the highly limited surface modiﬁcation or charge introduction by the enzyme. To evaluate distribution of the charged groups on the surfaces of CNs, zeta potentials of the CNs dispersed in water were investigated (Section 2.4.3). TCN displayed the highest charge density, with a zeta potential of −40.3 mV, and ACN displayed a charge density of −18.3 mV followed by slightly charged ECN (−7.48 mV (Table 1)). The high amount of charged groups and high zeta potential values indicate that the TCN and ACN dispersions in water will be very stable. For ECN, the zeta potential was quite low which conﬁrmed no extra charge introduction by the enzyme. It should be pointed out here that due to the longest length of ECN compared with ACN and TCN
Fig. 1. Characterisation of the freeze-dried cellulose nanocrystals against original cellulose and regenerated cellulose from tunicate. (A) FTIR spectra, (B) AFM images, (C) X-ray diffraction (XRD) patterns and (D) thermal gravimetric analysis (TGA) graphs.
Y. Zhao et al. / Carbohydrate Polymers 117 (2015) 286–296
(Table 1), there could be underestimation of the apparent value of zeta potential for ECN because larger particles moved slower. Furthermore, it is noticeable that the order for zeta potentials is consistent to that of charged group contents of CNs. It was conﬁrmed that different methods for preparation of CNs did lead to different charge density and distribution which may thus inﬂuence their behaviours in further applications. Obviously the TEMPO oxidation has been demonstrated to be the most effective method to introduce charges onto the surface of CN. Irrespective of the preparation method used, all of the CNs obtained were rod-like nanocrystals (Fig. 1(B)), displaying nanometre scale diameters, ranging from 15.9 to 20.2 nm. Although no signiﬁcant difference was observed in the width of the crystals among different CNs, the length decreases in the following order: ECN > TCN > ACN (by several micrometres, 1590 nm and 694 nm, respectively) (Table 1). In the literature, no systematic investigation or comparison has been reported for preparations of different CNs from TC with different methods. Generally, the sizes of TCNs in this study agree quite well with the reported values from different studies, e.g. ﬁbril length of 0.1–10 m and width of 5–20 nm (Habibi et al., 2006), and the ACN ﬁbrils having 1–2 m for length and 8–30 nm for width when obtained from other tunicate celluloses (Elazzouzi-Hafraoui et al., 2007; Rusli et al., 2011; Uddin, Araki, & Gotoh, 2011). All the CNs displayed similar morphology and crystallinity compared to the original TC due to limited modiﬁcations at the amorphous domains and the intact crystalline domains. As illustrated in Fig. 1(C), the X-ray diffraction curves of ECN, TCN and ACN displayed a typical cellulose I structure, with strong crystalline peaks at 14.7◦ , 16.8◦ and 22.8◦ , corresponding to the 1 1¯ 0 , (1 1 0), and (2 0 0) crystal planes, respectively. The crystallinity index (CI) increased in the following order: ECN < TCN < ACN (82.8, 87.5 and 90.7%, respectively). Thus, the higher the hydrolysis percentage during the CN preparation, the lower the extent of the remaining amorphous regions, resulting in the shorter length and the higher crystallinity of the CN. This ﬁnding could serve as a rule-of-thumb for the preparation of CNs. Comparatively, ECN has the highest thermal stability, as its decomposition started at approximately 260 ◦ C, the same temperature as for the starting TC (Fig. 1(D)). The decomposition of TCN began at approximately 220 ◦ C, 40 ◦ C lower than ECN, and ACN decomposed at a much lower temperature, ∼120 ◦ C. Apparently, the molecular mass is a decisive factor for thermal stability; the higher the Mw , the more thermally stable the CN. Notably, the CN crystallinity is not a decisive factor because the crystal structure in the regenerated TC has been mostly destroyed during the regeneration process but it still displayed good thermal stability. 3.3. CN ﬁlms In this study, the basic procedure for making CN ﬁlms was as follows: CN water suspension – casting – evaporation; this procedure is suitable for water soluble or dispersible polymers. After homogenisation and ultrasonication (see Section 2.2), all CNs were uniformly dispersed, especially TCN and ACN where the charged groups supplied additional electrostatic repulsion that assisted particle dispersion. Due to the dispersions, CN ﬁbrils have ultra-large interfacial areas. After casting in a very dilute concentration (0.5%), the CN ﬁbrils were randomly oriented in the dilute regime, and they arranged themselves as polymer lattices with the lowest repulsion after casting and evaporation. In addition, the evaporation of water tended to cause the CN ﬁbrils to adopt the conﬁguration that minimised electrostatic interactions, especially for TCN and ACN. In other words, the evaporation process was a self-assembly process used by the CN ﬁbrils to form an intermingling network structure. The thickness of the CN ﬁlms ranged from 10 to 20 m. The
Table 2 Speciﬁc surface area (m2 /g) of different neat CN and CN–GM ﬁlms.
After freeze drying Neat CN ﬁlm CN–KGM ﬁlm CN–SGM ﬁlm
161.3 29.0 18.7 (EKG30) 10.4 (ESG20)
61.7 61.1 4.40 (TKG50) 8.71 (TSG50)
26.0 63.4 3.70 (AKG50) 3.60 (ASG50)
rod-like CN ﬁbrils oriented themselves during network formation, and due to the high charges at the surface of TCN and ACN, the ﬁbrils tended to stretch and align parallel to each other, and this structure was preserved after complete water evaporation to form the ﬁlm (Fig. 2). During ﬁlm formation, interactions or inter-molecular hydrogen bonds are formed between the CN ﬁbrils as they approach each other. As a reference experiment, the CN suspensions were freeze-dried, and their speciﬁc surface areas (SSAs) were measured (Table 2). During freeze-drying, the water evaporated directly from ice without collapsing the structure of the network. Therefore, the SSA reﬂects the “original” distances between the CN ﬁbrils when no additional interaction was formed between the ﬁbrils. The CNs connected to each other with a SSA spacing of 161.3, 61.7 and 26.0 m2 /g for ECN, TCN and ACN, respectively. In contrast, the ECN ﬁlm formed after casting-evaporation was obviously denser than the “original” CN ﬁbrils, with a smaller SSA (28.9 vs. 161.3 m2 /g). The TCN ﬁlm had the similar SSA (61.1 vs. 61.7 m2 /g), while the ACN ﬁlm was more expanded (63.4 vs. 26.0 m2 /g) (Table 2). Apparently, ECN ﬁbrils tended to aggregate when the ﬁlm was forming. Due to their high charge, similar aggregations did not occur with TCN or ACN ﬁbrils. The TCN ﬁlm formed a similar network to that obtained after freeze-drying. For the ACN ﬁlm, a looser network was formed. 3.4. CN–GM composite ﬁlms The procedure of “water suspension–casting–evaporation” was also applied to prepare CN–GM composite ﬁlms after blending CN with GM during the ﬁrst step, when GM solution (for KGM) or suspension (for SGM) was added to the CN suspension. Due to similar polysaccharide structures, both CN and GM components display high density hydroxyl groups, which provide their hydrophilic nature and good miscibility and interactions (e.g., hydrogen bonds between the components are expected). After casting and evaporation, they formed the percolation network, with GM functioning as cement to reinforce the CN network in the composite ﬁlm. The thickness of the composite ﬁlms ranged from 10 to 20 m. The inter-ﬁbril interactions between CN and GM were observed using dynamic FTIR analysis of the EKG20 composite ﬁlm (Fig. 3) recorded at 0◦ polarisation, 80% RH and 30 ◦ C; the in-phase spectrum (thin line) indicates elastic responses, and the out-of-phase spectrum (thick line) indicates viscous responses. In the in-phase spectrum, two absorption vibrations are highlighted, one cellulose signal at 1434 cm−1 (C OH bending vibration of the CH2 OH group attached at glucose unit) and one KGM signal at 813 cm−1 caused by the equatorially aligned hydrogen at the C2 atom in the mannose residue, and they were simultaneously strained by the sinusoidal perturbation (Stevanic et al., 2012; Stevanic & Salmén, 2009). Interestingly, the interactions were observed at 80% RH and it resulted from the hydrogen bonds formed between ECN and KGM. Because of the strong interactions between CN and GM, the crystallinity index (CI) of the composite ﬁlms changed, as revealed by XRD analysis (Fig. 4(A)). The CI of all the CN composite ﬁlms with KGM decreased as the percentage of KGM increased. The strongest interactions were observed for ECN, which was the least charged of all the CNs. The CI for EKG ﬁlms decreased quickly (from 77% to 37%) when the KGM addition percentage increased from 0 to 50%.
Y. Zhao et al. / Carbohydrate Polymers 117 (2015) 286–296
Fig. 2. Surface SEM images and ﬁbril width distribution of CN or CN–GM composite ﬁlms.
Y. Zhao et al. / Carbohydrate Polymers 117 (2015) 286–296
Fig. 3. Dynamic FTIR spectra of EKG20 composite ﬁlm.
However, the changes for the TCN and ACN ﬁlms were not significant, except when the KGM percentage increased from 40 to 50% in the ACN composite ﬁlm. During composite ﬁlm formation, most of the cellulosic chains were perturbed by the presence of KGM, which decreased the crystallinity, verifying the results of another study (Whitney et al., 1998). In addition, this CI decrease could also be due to the masking effect from the added GM on the diffraction from the crystalline CNs. The strong interaction between CN and GM was conﬁrmed by measuring the width distribution of the CN microﬁbrils obtained from 100 measurements from multiple SEM images for each type of CN–GM composite ﬁlm (Fig. 2). Generally, the addition of GM increased the diameter of the majority of the ﬁbrils. For example, most of the ﬁbrils in the ECN neat ﬁlm were